# Toward nanofluids of ultra-high thermal conductivity

- 6.5k Downloads
- 13 Citations

**Part of the following topical collections:**

## Abstract

The assessment of proposed origins for thermal conductivity enhancement in nanofluids signifies the importance of particle morphology and coupled transport in determining nanofluid heat conduction and thermal conductivity. The success of developing nanofluids of superior conductivity depends thus very much on our understanding and manipulation of the morphology and the coupled transport. Nanofluids with conductivity of upper Hashin-Shtrikman (H-S) bound can be obtained by manipulating particles into an interconnected configuration that disperses the base fluid and thus significantly enhancing the particle-fluid interfacial energy transport. Nanofluids with conductivity higher than the upper H-S bound could also be developed by manipulating the coupled transport among various transport processes, and thus the nature of heat conduction in nanofluids. While the direct contributions of ordered liquid layer and particle Brownian motion to the nanofluid conductivity are negligible, their indirect effects can be significant via their influence on the particle morphology and/or the coupled transport.

## Keywords

Liquid Layer Effective Thermal Conductivity Base Fluid Thermal Wave Particle Volume Fraction## Abbreviations

- DPL
dual-phase-lagging

- H-S
Hashin-Shtrikman.

## Introduction

Nanofluids are a new class of fluids engineered by dispersing nanometer-size structures (particles, fibers, tubes, droplets, etc.) in base fluids. The very essence of nanofluids research and development is to enhance fluid macroscopic and system-scale properties through manipulating microscopic physics (structures, properties, and activities) [1, 2]. One of such properties is the thermal conductivity that characterizes the strength of heat conduction and has become a research focus of nanofluid society in the last decade [1, 2, 3, 4, 5, 6, 7, 8, 9].

The importance of high-conductivity nanofluids cannot be overemphasized. The success of effectively developing such nanofluids depends very much on our understanding of mechanism responsible for the significant enhancement of thermal conductivity. Both static and dynamic reasons have been proposed for experimental finding of significant conductivity enhancement [1, 2, 3, 4, 5, 6, 7, 8, 9]. The former includes the nanoparticle morphology [10, 11] and the liquid layering at the liquid-particle interface [12, 13, 14, 15, 16, 17]. The latter contains the coupled (cross) transport [18, 19, 20] and the nanoparticle Brownian motion [21, 22, 23, 24, 25, 26]. Here, the effect of particle morphology contains those from the particle shape, connectivity among particles (including and generalizing the nanoparticle clustering/aggregating in the literature [10, 11]), and particle distribution in nanofluids. This short review aims for a concise assessment of these contributions, thus identifying the future research needs toward nanofluids of high thermal conductivity. The readers are referred to, for example, [1, 2, 3, 4, 5, 6, 7, 8, 9] for state-of-the-art expositions of major advances on the synthesis, characterization, and application of nanofluids.

### Static mechanisms

#### Morphology

The nanoparticle morphology in nanofluids can vary from a well-dispersed configuration in base fluids to a continuous phase of interconnected configuration. Such a morphology variation will change nanofluid's effective thermal conductivity significantly [27, 28, 29, 30, 31, 32], a phenomenon credited to the particle clustering/aggregating in the literature [1, 2, 3, 4, 5, 6, 7, 8, 9]. This appears obvious because the nanofluid's effective conductivity stems mainly from the contribution of continuous phase that constitutes the continuous path for thermal flow [27, 28]. Although particle clustering/aggregating offers a way of changing particle morphology, it is not necessarily an effective means. The research should thus focus not only on the clustering/aggregating, but also on the general ways of varying morphology.

Here *k*_{p}, *k*_{f}, and *k*_{e} are the conductivities of particle, base fluid, and nanofluid, respectively, and *φ* is the particle volume fraction. For the case of *k*_{p}/*k*_{f} ≥1, Equations (1) and (2) give the lower and the upper bounds for nanofluid effective thermal conductivity, corresponding to the two limiting morphologies where the liquid serves as the continuous phase for the lower bound and the particle disperses the liquid for the upper bound, respectively. When *k*_{p}/*k*_{f} ≤1, their roles are interchanged, so that Equations (1) and (2) provide the upper and the lower bounds, respectively. Therefore, the upper bound always takes a configuration (morphology) where the continuous phase is made of the higher-conductivity material.

The morphology dependence of nanofluid's conductivity has been recently examined in detail by either of the two approaches: the constructal approach [1, 2, 29, 30, 31, 32] and the scaling-up by the volume average [1, 2, 27, 28]. Such studies not only confirm the features captured in the H-S bounds but also uncover the microscopic mechanism responsible for the morphology dependence of nanofluid's conductivity. As higher-conductivity particles interconnect each other and disperse the lower-conductivity base fluid into a dispersed phase, the interfacial energy transport between particle and base fluid becomes enhanced significantly such that the nanofluid's conductivity takes its value of upper H-S bound (Fan J and Wang LQ: Heat conduction in nanofluids: structure-property correlation, submitted).

As *k*_{p}/*k*_{f} moves away from the unity along both directions, the separation between the upper and lower H-S bounds becomes pronounced (Figures 1 and 2) so that the room for manipulating nanofluid conductivity via changing the particle morphology becomes more spacious. The H-S bounds are respected by some nanofluids for which their thermal conductivity is strongly dependent on particle morphology, such as whether nanoparticles stay well-dispersed in the base fluid, form aggregates, or assume a configuration of continuous phase that disperses the fluid into a dispersed phase (Figure 1). There are thermal conductivity data that fall outside the H-S bounds (Figures 1 and 2).

#### Ordered liquid layer

Both experimental and theoretical evidences have been reported of the presence of ordered liquid layer near a solid surface by which the atomic structure of the liquid layer is significantly more ordered than that of bulk liquid [64, 65, 66, 67]. For example, two layers of icelike structures are experimentally observed to be strongly bounded to the crystal surface on a crystal-water interface, followed by two diffusive layers with less significant ordering [65]. Three ordered water layers have also been observed numerically on the Pt (111) surface [64].

*h*of such liquid layers around the solid surface can be estimated by [17]

where *N*_{a} is the Avogadro's number, and *ρ*_{f} and *M*_{f} are the density and the molecular weight of base fluids, respectively. The liquid layer thickness is thus 0.28 nm for water-based nanofluids, which agrees with that from experiments and molecular dynamic simulation on the order of magnitude.

*d*

_{p}, Equation (1) offers the conductivity ratio with and without this effect:

*η*= (

*k*

_{p}-

*k*

_{f})/(

*k*

_{p}+ 2

*k*

_{f}). The variation of (

*k*

_{e})

_{with}/(

*k*

_{e})

_{without}with

*ηφ*and

*d*

_{p}/2

*h*is illustrated in Figure 3, showing that the liquid-layering effect is important only when

*ηφ*is large and

*d*

_{p}/2

*h*is small. This is normally not the case for practical nanofluids. For Cu-in-water nanofluids (η ≈ 1), for example, (

*k*

_{e})

_{with}/(

*k*

_{e})

_{without}≈ 1.005 with

*φ*= 0.5% and

*d*

_{p}= 10 nm.

### Dynamic mechanisms

#### Coupled transport

In a nanofluid system, normally, there are two or more transport processes that occur simultaneously. Examples are the heat conduction in dispersed phase, heat conduction in continuous phase, mass transport, and chemical reactions either among the nanoparticles or between the nanoparticles and the base fluid. These processes may couple (interfere) and cause new induced effects of flows occurring without or against its primary thermodynamic driving force, which may be a gradient of temperature, or chemical potential, or reaction affinity. Two classical examples of coupled transport are the Soret effect (also known as thermodiffusion or thermophoresis) in which directed motion of particles or macromolecules is driven by thermal gradient and the Dufour effect that is an induced heat flow caused by the concentration gradient.

*β*and

*σ-*phases, respectively, the temperature

*T*obeys the following energy equations [1, 2]

where *T* is the temperature; subscripts *β* and *σ* refer to the *β* and *σ-* phases, respectively. *γ*_{ β }= (1 - *φ*)(*ρc*)*β* and *γ*_{ σ }= *φ*(*ρc*)_{ σ }are the effective thermal capacities of *β* and *σ-* phases, respectively, with *ρ* and *c* as the density and the specific heat. *φ* is the volume fraction of the *σ-* phase. *h* and *a*_{ υ }come from modeling of the interfacial flux and are the film heat transfer coefficient and the interfacial area per unit volume, respectively. *k*_{ ββ }and *k*_{ σσ }are the effective thermal conductivities of the *β* and *σ-* phases, respectively; *k*_{ βσ }and *k*_{ σβ }are the coupling (cross) effective thermal conductivities between the two phases.

*i*can take

*β*or

*σ*. Its explicit form reads, after dividing by

*ha*

_{υ}(

*γ*

_{ β }+

*γ*

_{ σ })

Equation (12) is not a classical heat-conduction equation, but can be regarded as a dual-phase-lagging (DPL) heat-conduction equation with ((*k*_{ βσ }*k*_{ σβ }- *k*_{ ββ }*k*_{ σσ })/(*ha*_{ υ }))Δ^{2}*T*_{ i }as the DPL source-related term $F(\text{r},t)+{\tau}_{q}\frac{\partial F(\text{r},t)}{\partial t}$ and with *τ*_{ q }and *τ*_{ T }as the phase lags of the heat flux and the temperature gradient, respectively [2, 18, 69]. Here, *F*(r, *t*) is the volumetric heat source. *k*, *ρc*, and *α* are the effective thermal conductivity, capacity and diffusivity of nanofluids, respectively.

*k*

_{ ββ },

*k*

_{ σσ },

*k*

_{ βσ }, and

*k*

_{ σβ }are available in [27, 28] for some typical nanofluids. The coupled-transport contribution to the nanofluid thermal conductivity, the term (

*k*

_{ βσ }+

*k*

_{ σβ }), can be as high as 10% of the of the overall thermal conductivity [27, 28]. The more striking effect of the coupled transport on nanofluid heat conduction can be found by considering

Therefore, by the condition for the existence of thermal waves that requires *τ*_{ T }/*τ*_{ q }*<* 1 [18, 70], thermal waves may be present in nanofluid heat conduction.

Note also that, for heat conduction in nanofluids, there is a time-dependent source term *F*(r, *t*) in the DPL heat conduction (Equations (12) and (13)). Therefore, the resonance can also occur. When *k*_{ βσ }= *k*_{ σβ }= 0 so that *τ*_{ T }/*τ*_{ q }is always larger than 1, thermal waves and resonance would not appear. Therefore, the coupled transport could change the nature of heat conduction in nanofluids from a diffusion process to a wave process, thus having a significant effect on nanofluid heat conduction.

Therefore, the cross coupling between the heat conduction in the fluid and particle manifests itself as thermal waves at the macroscale. Depending on factors such as material properties of nanoparticles and base fluids, nanoparticles' geometrical structure and their distribution in the base fluids, and interfacial properties and dynamic processes on particle-fluid interfaces, the cross-coupling-induced thermal waves may either enhance or counteract with the molecular-dynamics-driven heat diffusion. Consequently, the heat conduction may be enhanced or weakened by the presence of nanoparticles. This explains the thermal conductivity data that fall outside the H-S bounds (Figures 1 and 2).

*T*and particle volume fraction

*φ*satisfy the following equations of energy and mass conservation:

*D*

_{ σσ }is the effective diffusion coefficient for nanoparticles.

*k*

_{β m},

*k*

_{σ m},

*D*

_{mβ},

*D*

_{mσ}, and

*D*

_{mT}are five transport coefficients for coupled heat and mass transport. By following a similar procedure as that of developing Equation (12), an uncoupled form with

*u*(

*T*

_{ β },

*T*

_{ σ }, or

*φ*) as the sole unknown variable is obtained,

This can be regarded as a DPL heat-conduction equation regarding Δ*u* with *τ*_{ q }*, τ*_{ T }, and $F(\text{r},t)+{\tau}_{q}\frac{\partial F(\text{r},t)}{\partial t}$ as the phase lags of the heat flux and the temperature gradient, and the source-related term, respectively. Therefore, the coupled heat and mass transport is capable of varying not only thermal conductivity from that in Equation (13) to the one in Equation (21) but also the nature of heat conduction from that in Equation (12) to the one in Equation (19). As practical nanofluid system always involves many transport processes simultaneously, the coupled transport could play a significant role. For assessing its effect and understanding heat conduction in nanofluids, future research is in great demand on coupling (cross) transport coefficients that are derivable by approaches like the up-scaling with closures [2, 27, 28], the kinetic theory [71, 72], the time-correlation functions [73, 74], and the experiments based on phenomenological flux relations [68]. While the uncoupled form of conservation equations, such as Equations (12) and (19), is very useful for examining nature of heat transport, its coupled form, such as Equations (8), (9), (16)-(18), is normally more readily to be resolved for the temperature or concentration fields after all the transport coefficients are available.

#### Brownian motion

*k*

_{BD}) to the base fluid conductivity (

*k*

_{f}) is estimated based on the kinetic theory [75],

*k*

_{B}is the Boltzmann's constant (1.38065 × 10

^{-23}J/K); and

*μ*is the fluid viscosity. The kinetic theory also gives an upper limit for the ratio of the latter's contribution to the thermal conductivity (

*k*

_{BC}) to the base fluid conductivity (

*k*

_{f}) [76],

where subscript BC refers to the Brownian-motion-induced convection, and *α*_{f} is the thermal diffusivity of the base fluid.

Consider a 1% volume fraction of *d*_{p} = 10 nm copper nanoparticle in water suspension at *T* = 300 K. (*ρc*)_{P} = 8900 kg/m^{3} × 0.386 kJ/(kg K) = 3435.4 kJ/(m^{3} K), μ = 0.798 × 10^{-3}kg/(ms), *k*_{f} = 0.615 W/(mK), and *α*_{f} = 1.478 × 10^{-7} m^{2}/s. These yield *k*_{BD}/*k*_{f} = 3.076 × 10^{-6} and *k*_{BC}/*k*_{f} = 3.726 × 10^{-4}. Therefore, both contributions are negligibly small.

Although the direct contribution of particle Brownian motion to the nanofluid conductivity is negligible, its indirect effect could be significant because it plays an important role in processes of particle aggregating and coupled transport.

## Concluding remarks

Under the specified volume fractions and thermal conductivities of the two phases in the colloidal state, the interfacial energy transport between the two phases favors a configuration in which the higher-conductivity phase forms a continuous path for thermal flow and disperses the lower-conductivity phase. The effective thermal conductivity is thus bounded by those corresponding to the two limiting morphologies: the well-dispersed configuration of the higher-conductivity phase in the lower-conductivity phase and the well-dispersed configuration of the lower-conductivity phase in the higher-conductivity phase, corresponding to the lower and the upper bounds of thermal conductivity, respectively. Without considering the effect of interfacial resistance and cross coupling among various transport processes, the classical effective-medium theory gives these bounds known as the H-S bounds. A wide separation of these two bounds offers spacious room of manipulating nanofluid thermal conductivity via the morphology effect.

In a nanofluid system, there are normally two or more transport processes that occur simultaneously. The cross coupling among these processes causes new induced effects of flows occurring without or against its primary thermodynamic driving force and is capable of changing the nature of heat conduction via inducing thermal waves and resonance. Depending on the microscale physics (factors like material properties of nanoparticles and base fluids, nanoparticles' morphology in the base fluids, and interfacial properties and dynamic processes on particle-fluid interfaces), the heat diffusion and thermal waves may either enhance or counteract each other. Consequently, the heat conduction may be enhanced or weakened by the presence of nanoparticles.

The direct contributions of ordered liquid layer and particle Brownian motion to the nanofluid conductivity are negligible. Their influence on the particle morphology and/or the coupled transport could, however, offer a strong indirect effect to the nanofluid conductivity.

Therefore, nanofluids with conductivity of upper H-S bound can be obtained by manipulating particles into an interconnected configuration that disperses the base fluid, and thus significantly enhancing the particle-fluid interfacial energy transport. Nanofluids with conductivity higher than the upper H-S bound could also be developed by manipulating the cross coupling among various transport processes and thus the nature of heat conduction in nanofluids.

## Notes

### Acknowledgements

The financial support from the Research Grants Council of Hong Kong (GRF718009 and GRF717508) is gratefully acknowledged.

## Supplementary material

## References

- 1.Wang LQ, Fan J: Nanofluids Research: Key Issues.
*Nanoscale Res Lett*2010, 5: 1241. 10.1007/s11671-010-9638-6CrossRefGoogle Scholar - 2.Wang LQ, Quintard M: Nanofluids of the future. In
*Advances in Transport Phenomena*. New York: Springer; 2009:179. 2009 2009 full_textCrossRefGoogle Scholar - 3.Choi SUS, Zhang ZG, Keblinski P: Nanofluids. In
*Encyclopedia of Nanoscience and Nanotechnology*. Edited by: Nalwa HS. New York: American Scientific Publishers; 2004:757.Google Scholar - 4.Peterson GP, Li CH: Heat and mass transfer in fluids with nanoparticle suspensions.
*Adv Heat Transfer*2006, 39: 257. full_textCrossRefGoogle Scholar - 5.Das CH, Choi SUS, Yu W, Pradeep T:
*Nanofluids: Science and Technology*. Hoboken, NJ: John Wiley & Sons, Inc; 2008.Google Scholar - 6.Sobhan CB, Peterson GP:
*Microscale and Nanoscale Heat Transfer: Fundamentals and Engineering Applications*. Boca Raton: CRC Press; 2008.Google Scholar - 7.Choi SUS: Nanofluids: from vision to reality through research.
*ASME J Heat Transfer*2009, 131: 033106. 10.1115/1.3056479CrossRefGoogle Scholar - 8.Fan J, Wang LQ: Review of heat conduction in nanofluids.
*ASME J Heat Transfer*2011, 133: 040801. 10.1115/1.4002633CrossRefGoogle Scholar - 9.Wang LQ, Wei XH: Heat conduction in nanofluids. In
*Handbook of Nanophysics: Nanoparticles and Quantum Dots*.*Volume Chapter 33*. Edited by: Sattler K. Taylor & Francis; 2010:33–1.Google Scholar - 10.Prasher R, Phelan PE, Bhattacharya P: Effect of aggregation kinetics on the thermal conductivity of nanoscale colloidal solutions (Nanofluids).
*Nano Lett*2006, 6: 1529. 10.1021/nl060992sCrossRefGoogle Scholar - 11.Rusconi R, Rodari E, Piazza R: Optical measurements of the thermal properties of nanofluids.
*Appl Phys Lett*2006, 89: 261916. 10.1063/1.2425015CrossRefGoogle Scholar - 12.Yu W, Choi SUS: The role of interfacial layers in the enhanced thermal conductivity of nanofluids: A renovated Hamilton-Crosser model.
*J Nanopart Res*2004, 6: 355. 10.1007/s11051-004-2601-7CrossRefGoogle Scholar - 13.Xue L, Keblinski P, Phillpot SR, Choi SUS, Eastman JA: Effect of liquid layering at the liquid-solid interface on thermal transport.
*Int J Heat Mass Transfer*2004, 47: 4277. 10.1016/j.ijheatmasstransfer.2004.05.016CrossRefGoogle Scholar - 14.Xie HQ, Fujii M, Zhang X: Effect of interfacial nanolayer on the effective thermal conductivity of nanoparticle-fluid mixture.
*Int J Heat Mass Transfer*2005, 48: 2926. 10.1016/j.ijheatmasstransfer.2004.10.040CrossRefGoogle Scholar - 15.Ren Y, Xie H, Cai A: Effective thermal conductivity of nanofluids containing spherical nanoparticles.
*J Phys D Appl Phys*2005, 38: 3958. 10.1088/0022-3727/38/21/019CrossRefGoogle Scholar - 16.Leong KC, Yang C, Murshed SMS: A model for the thermal conductivity of nanofluids - the effect of interfacial layer.
*J Nanopart Res*2006, 8: 245. 10.1007/s11051-005-9018-9CrossRefGoogle Scholar - 17.Wang BX, Zhou LP, Peng XF: A fractal model for predicting the effective thermal conductivity of liquid with suspension of nanoparticles.
*Int J Heat Mass Transfer*2003, 46: 2665. 10.1016/S0017-9310(03)00016-4CrossRefGoogle Scholar - 18.Wang LQ, Zhou XS, Wei XH:
*Heat Conduction: Mathematical Models and Analytical Solutions*. Heidelberg, Berlin: Springer-Verlag; 2008.Google Scholar - 19.Wang LQ, Xu MT, Wei XH: Multiscale theorems.
*Adv Chem Eng*2008, 34: 175. full_textCrossRefGoogle Scholar - 20.Wang L, Wei X: Nanofluids: synthesis, heat conduction, and extension.
*ASME J Heat Transfer*2009, 131: 033102. 10.1115/1.3056597CrossRefGoogle Scholar - 21.Koo J, Kleinstreuer C: A new thermal conductivity model for nanofluids.
*J Nanopart Res*2004, 6: 577. 10.1007/s11051-004-3170-5CrossRefGoogle Scholar - 22.Jang SP, Choi SUS: Role of Brownian motion in the enhanced thermal conductivity of nanofluids.
*Appl Phys Lett*2004, 84: 4316. 10.1063/1.1756684CrossRefGoogle Scholar - 23.Bhattacharya P, Saha SK, Yadav A, Phelan PE, Prasher RS: Brownian dynamics simulation to determine the effective thermal conductivity of nanofluids.
*J Appl Phys*2004, 95: 6492. 10.1063/1.1736319CrossRefGoogle Scholar - 24.Prasher R, Bhattacharya P, Phelan P: Thermal conductivity of nanoscale colloidal solutions (nanofluids).
*Phys Rev Lett*2005, 94: 025901. 10.1103/PhysRevLett.94.025901CrossRefGoogle Scholar - 25.Prasher R, Bhattacharya P, Phelan PE: Brownian-motion-based convective-conductive model for the effective thermal conductivity of nanofluids.
*J Heat Transfer Trans ASME*2006, 128: 588. 10.1115/1.2188509CrossRefGoogle Scholar - 26.Yu W, Choi SUS: The role of interfacial layers in the enhanced thermal conductivity of nanofluids: A renovated Maxwell model.
*J Nanopart Res*2003, 5: 167. 10.1023/A:1024438603801CrossRefGoogle Scholar - 27.Fan J, Wang LQ: Effective thermal conductivity of nanofluids: the effects of microstructure.
*J Phys D Appl Phys*2010, 43: 165501. 10.1088/0022-3727/43/16/165501CrossRefGoogle Scholar - 28.Fan J, Wang LQ: Microstructural effects on macroscale thermal properties in nanofluids.
*NANO*2010, 5: 117. 10.1142/S1793292010002001CrossRefGoogle Scholar - 29.Fan J, Wang LQ: Constructal design of nanofluids.
*Int J Heat Mass Transfer*2010, 53: 4238. 10.1016/j.ijheatmasstransfer.2010.05.050CrossRefGoogle Scholar - 30.Bai C, Wang LQ: Constructal structure of nanofluids.
*J Appl Phys*2010, 108: 068979.Google Scholar - 31.Bai C, Wang LQ: Constructal Allocation of Nanoparticles in Nanofluids.
*J Heat Transfer Trans ASME*2010, 132: 052404. 10.1115/1.4000473CrossRefGoogle Scholar - 32.Bai C, Wang LQ: Constructal design of nanofluids for one-dimensional steady heat conduction systems.
*NANO*2010, 5: 39. 10.1142/S1793292010001895CrossRefGoogle Scholar - 33.Hashin Z, Shtrikman S: A variational approach to the theory of the effective magnetic permeability of multiphase materials.
*J Appl Phys*1962, 33: 3125. 10.1063/1.1728579CrossRefGoogle Scholar - 34.Wei XH, Wang LQ: 1+1 > 2: Extraordinary fluid conductivity enhancement.
*Curr Nanosci*2009, 5: 527.CrossRefGoogle Scholar - 35.Kang HU, Kim SH, Oh JM: Estimation of thermal conductivity of nanofluid using experimental effective particle volume.
*Exp Heat Transfer*2006, 19: 181. 10.1080/08916150600619281CrossRefGoogle Scholar - 36.Eapen J, Li J, Yip S: Mechanism of thermal transport in dilute nanocolloids.
*Phys Rev Lett*2007, 98: 028302. 10.1103/PhysRevLett.98.028302CrossRefGoogle Scholar - 37.Buongiorno J, Venerus DC, Prabhat N, McKrell T, Townsend J, Christianson R, Tolmachev YV, Keblinski P, Hu LW, Alvarado JL, Bang IC, Bishnoi SW, Bonetti M, Botz F, Cecere A, Chang Y, Chen G, Chen HS, Chung SJ, Chyu MK, Das SK, Di Paola R, Ding YL, Dubois F, Dzido G, Eapen J, Escher W, Funfschilling D, Galand Q, Gao JW, Gharagozloo PE, Goodson KE, Gutierrez JG, Hong HP, Horton M, Hwang KS, Iorio CS, Jang SP, Jarzebski AB, Jiang YR, Jin LW, Kabelac S, Kamath A, Kedzierski MA, Kieng LG, Kim C, Kim JH, Kim S, Lee SH, Leong KC, Manna I, Michel B, Ni R, Patel HE, Philip J, Poulikakos D, Reynaud C, Savino R, Singh PK, Song PX, Sundararajan T, Timofeeva E, Tritcak T, Turanov AN, Van Vaerenbergh S, Wen DS, Witharana S, Yang C, Yeh WH, Zhao WH, Zhou SQ: A benchmark study on the thermal conductivity of nanofluids.
*J Appl Phys*2009, 106: 094312. 10.1063/1.3245330CrossRefGoogle Scholar - 38.Williams W, Buongiorno J, Hu LW: Experimental investigation of turbulent convective heat transfer and pressure loss of alumina/water and zirconia/water nanoparticle colloids (nanofluids) in horizontal tubes.
*J Heat Transfer Trans ASME*2008, 130: 042412. 10.1115/1.2818775CrossRefGoogle Scholar - 39.Zhang X, Gu H, Fujii M: Experimental study on the effective thermal conductivity and thermal diffusivity of nanofluids.
*Int J Thermophys*2006, 27: 569. 10.1007/s10765-006-0054-1CrossRefGoogle Scholar - 40.Zhu HT, Zhang CY, Liu SQ, Tang YM, Yin YS: Effects of nanoparticle clustering and alignment on thermal conductivities of Fe3O4 aqueous nanofluids.
*Appl Phys Lett*2006, 89: 023123. 10.1063/1.2221905CrossRefGoogle Scholar - 41.Shima PD, Philip J, Raj B: Role of microconvection induced by Brownian motion of nanoparticles in the enhanced thermal conductivity of stable nanofluids.
*Appl Phys Lett*2009, 94: 223101. 10.1063/1.3147855CrossRefGoogle Scholar - 42.Murshed SMS, Leong KC, Yang C: Enhanced thermal conductivity of TiO2 - water based nanofluids.
*Int J Therm Sci*2005, 44: 367. 10.1016/j.ijthermalsci.2004.12.005CrossRefGoogle Scholar - 43.Duangthongsuk W, Wongwises S: Measurement of temperature-dependent thermal conductivity and viscosity of TiO2-water nanofluids.
*Exp Therm Fluid Sci*2009, 33: 706. 10.1016/j.expthermflusci.2009.01.005CrossRefGoogle Scholar - 44.Mintsa HA, Roy G, Nguyen CT, Doucet D: New temperature dependent thermal conductivity data for water-based nanofluids.
*Int J Therm Sci*2009, 48: 363. 10.1016/j.ijthermalsci.2008.03.009CrossRefGoogle Scholar - 45.Lee DY, Vafai K: Analytical characterization and conceptual assessment of solid and fluid temperature differentials in porous media.
*Int J Heat Mass Transfer*1999, 42: 423. 10.1016/S0017-9310(98)00185-9CrossRefGoogle Scholar - 46.Das SK, Putra N, Thiesen P, Roetzel W: Temperature dependence of thermal conductivity enhancement for nanofluids.
*ASME J Heat Transfer*2003, 125: 567. 10.1115/1.1571080CrossRefGoogle Scholar - 47.Li CH, Peterson GP: Experimental investigation of temperature and volume fraction variations on the effective thermal conductivity of nanoparticle suspensions (nanofluids).
*J Appl Phys*2006, 99: 084314. 10.1063/1.2191571CrossRefGoogle Scholar - 48.Zhu HT, Zhang CY, Tang YM, Wang JX: Novel synthesis and thermal conductivity of CuO nanofluid.
*J Phys Chem C*2007, 111: 1646. 10.1021/jp065926tCrossRefGoogle Scholar - 49.Hong JG, Kim SH, Kim DS: Effect of laser irradiation on thermal conductivity of ZnO nanofluids.
*J Phys Conf Ser*2007, 59: 301. 10.1088/1742-6596/59/1/063CrossRefGoogle Scholar - 50.Kim SH, Choi SR, Kim D: Thermal conductivity of metal-oxide nanofluids: Particle size dependence and effect of laser irradiation.
*J Heat Transfer Trans ASME*2007, 129: 298. 10.1115/1.2427071CrossRefGoogle Scholar - 51.Wen DS, Ding YL: Experimental investigation into convective heat transfer of nanofluids at the entrance region under laminar flow conditions.
*Int J Heat Mass Transfer*2004, 47: 5181. 10.1016/j.ijheatmasstransfer.2004.07.012CrossRefGoogle Scholar - 52.Gharagozloo PE, Eaton JK, Goodson KE: Diffusion, aggregation, and the thermal conductivity of nanofluids.
*Appl Phys Lett*2008, 93: 103110. 10.1063/1.2977868CrossRefGoogle Scholar - 53.Moosavi M, Goharshadi EK, Youssefi A: Fabrication, characterization, and measurement of some physicochemical properties of ZnO nanofluids.
*Int J Heat Fluid Flow*2010, 31: 599. 10.1016/j.ijheatfluidflow.2010.01.011CrossRefGoogle Scholar - 54.Hong TK, Yang HS, Choi CJ: Study of the enhanced thermal conductivity of Fe nanofluids.
*J Appl Phys*2005, 97: 064311. 10.1063/1.1861145CrossRefGoogle Scholar - 55.Sinha K, Kavlicoglu B, Liu YM, Gordaninejad F, Graeve OA: A comparative study of thermal behavior of iron and copper nanofluids.
*J Appl Phys*2009, 106: 064307. 10.1063/1.3225574CrossRefGoogle Scholar - 56.Murshed SMS, Leong KC, Yang C: Determination of the effective thermal diffusivity of nanofluids by the double hot-wire technique.
*J Phys D Appl Phys*2006, 39: 5316. 10.1088/0022-3727/39/24/033CrossRefGoogle Scholar - 57.Eastman JA, Choi SUS, Li S, Yu W, Thompson LJ: Anomalously increased effective thermal conductivities of ethylene glycol-based nanofluids containing copper nanoparticles.
*Appl Phys Lett*2001, 78: 718. 10.1063/1.1341218CrossRefGoogle Scholar - 58.Assael MJ, Metaxa IN, Kakosimos K, Constantinou D: Thermal conductivity of nanofluids - experimental and theoretical.
*Int J Thermophys*2006, 27: 999. 10.1007/s10765-006-0078-6CrossRefGoogle Scholar - 59.Garg J, Poudel B, Chiesa M, Gordon JB, Ma JJ, Wang JB, Ren ZF, Kang YT, Ohtani H, Nanda J, McKinley GH, Chen G: Enhanced thermal conductivity and viscosity of copper nanoparticles in ethylene glycol nanofluid.
*J Appl Phys*2008, 103: 074301. 10.1063/1.2902483CrossRefGoogle Scholar - 60.Xie H, Lee H, Youn W, Choi M: Nanofluids containing multiwalled carbon nanotubes and their enhanced thermal conductivities.
*J Appl Phys*2003, 94: 4967. 10.1063/1.1613374CrossRefGoogle Scholar - 61.Liu MS, Lin MCC, Huang IT, Wang CC: Enhancement of thermal conductivity with carbon nanotube for nanofluids.
*Int Commun Heat Mass Transfer*2005, 32: 1202. 10.1016/j.icheatmasstransfer.2005.05.005CrossRefGoogle Scholar - 62.Choi SUS, Zhang ZG, Yu W, Lockwood FE, Grulke EA: Anomalous thermal conductivity enhancement in nanotube suspensions.
*Appl Phys Lett*2001, 79: 2252. 10.1063/1.1408272CrossRefGoogle Scholar - 63.Xie H, Wang J, Xi T, Liu Y, Ai F: Thermal conductivity enhancement of suspensions containing nanosized alumina particles.
*J Appl Phys*2002, 91: 4568. 10.1063/1.1454184CrossRefGoogle Scholar - 64.Raghavan K, Foster K, Motakabbir K, Berkowitz M: Structure and Dynamics of Water at the Pt(111) Interface - Molecular-Dynamics Study.
*J Chem Phys*1991, 94: 2110. 10.1063/1.459934CrossRefGoogle Scholar - 65.Reedijk MF, Arsic J, Hollander FFA, de Vries SA, Vlieg E: Liquid order at the interface of KDP crystals with water: Evidence for icelike layers.
*Phys Rev Lett*2003, 90: 066103. 10.1103/PhysRevLett.90.066103CrossRefGoogle Scholar - 66.Mo H, Evmenenko G, Dutta P: Ordering of liquid squalane near a solid surface.
*Chem Phys Lett*2005, 415: 106. 10.1016/j.cplett.2005.08.142CrossRefGoogle Scholar - 67.Yu CJ, Richter AG, Kmetko J, Dugan SW, Datta A, Dutta P: Structure of interfacial liquids: X-ray scattering studies.
*Phys Rev E*2001, 63: 021205. 10.1103/PhysRevE.63.021205CrossRefGoogle Scholar - 68.Demirel Y:
*Nonequilibrium Thermodynamics: Transport and Rate Processes in Physical, Chemical and Biological Systems*. 2nd edition. Amsterdam: Elsevier; 2007.Google Scholar - 69.Tzou D:
*Macro- to Micro-Scale Heat Transfer: The Lagging Behavior*. Washington, DC: Taylor & Francis; 1997.Google Scholar - 70.Xu MT, Wang LQ: Thermal oscillation and resonance in dual-phase-lagging heat conduction.
*Int J Heat Mass Transfer*2002, 45: 1055. 10.1016/S0017-9310(01)00199-5CrossRefGoogle Scholar - 71.Chapman S, Cowling TG:
*The Mathematical Theory of Non-Uniform Gases: An Account of the Kinetic Theory of Viscosity, Thermal Conduction and Diffusion in Gases*. Cambridge: Cambridge University Press; 1991.Google Scholar - 72.Hanley HJM:
*Transport Phenomena in Fluids*. New York: Marcel Dekker; 1969.Google Scholar - 73.McQuarrie DA:
*Statistical Mechanics*. Sausalito: University Science Books; 2000.Google Scholar - 74.Zwanzig RW: Time-correlation functions and transport coefficients in statistical mechanics.
*Annu Rev Phys Chem*1965, 16: 67. 10.1146/annurev.pc.16.100165.000435CrossRefGoogle Scholar - 75.Keblinski P, Cahil DG: Comment on "Model for heat conduction in nanofluids.
*Phys Rev Lett*2005, 95: 209401. 10.1103/PhysRevLett.95.209401CrossRefGoogle Scholar - 76.Evans W, Fish J, Keblinski P: Role of Brownian motion hydrodynamics on nanofluid thermal conductivity.
*Appl Phys Lett*2006, 88: 093116. 10.1063/1.2179118CrossRefGoogle Scholar

## Copyright information

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.